HEAT TREATMENT OF METALS 2004.1 p.11-15
From HEAT TREATMENT OF METALS, the quarterly journal of Wolfson Heat Treatment Centre, Aston University, Aston Triangle, Birmingham B4 7ET, UK at www.aston.ac.uk/whtc.
Induction Hardening of Gears: a ReviewV. RUDNEV, D. LOVELESS, R. COOK and M. BLACK Inductoheat Inc., USA Extracted from the authors new book* on induction heating, this comprehensive overview of gear hardening concludes by examining spin hardening with encircling inductors.
Part 2Gear Spin Hardening (Encircling Inductors) Spin hardening of gears utilises a single or multi-turn inductor that encircles the part and requires gear rotation. It is used typically for gears with fine- and medium-sized teeth and is considered less time-consuming and more costeffective than the previously-discussed processes. Therefore, the use of spin hardening is strongly recommended whenever it is possible. Unfortunately, spin hardening is not a cure-all and sometimes cannot be used easily for medium-sized helical and bevel gears and largemodule gears, due to an enormously-large amount of required power and difficulties in obtaining the desired hardness pattern. Gears are rotated during heating to ensure an even distribution of energy across their perimeter. Rotation rates are chosen to suit process requirements. When applying encircling coils, there are five parameters that play a dominant role in obtaining the required hardness pattern: frequency, power, cycle time, coil geometry and quenching conditions. Proper control of these parameters can result in totally different hardened profiles. Fig. 12 illustrates a diversity of induction hardening patterns that were obtained on the same carbon steel shaft with variations in time, frequency and power. As a basic*This is an edited version of a section from Handbook of Induction Heating, the new publication from Marcel Dekker (www.dekker.com), which is reviewed on pages 78-79 of the 2003.3 issue of HEAT TREATMENT OF METALS. Full details about the book appear on page v in this issue. The publishers kind permission to feature this extract here is gratefully acknowledged.(a) Conventional SingleFrequency Concept (CSFC)
Fig.12. Diversity of induction hardening patterns, with variations in time, frequency and power. (Courtesy of J. LaMonte, Inductoheat Inc.).
rule, when it is necessary to harden the tooth tips only, a higher frequency and high power density should be applied (Fig.4a). When hardening the tooth root, a lower frequency and lower power density should be employed (Fig.4b). A high power density generally gives a shallow pattern; conversely, a low power density will produce a deep pattern. In addition to the process parameters mentioned above, hardness pattern uniformity and repeatability depend strongly upon the relative positioning of gear and coil and the ability to maintain gear concentricity within the induction coil. There are several ways to accomplish quenching in spin hardening of gears. One technique is to submerge the gear in a quenching tank. This is applicable for large-size gears. Gears of small and medium size are usually quenched in(c) Pulsing Dual-Frequency Concept (PDFC)
(b) Pulsing Single-Frequency Concept (PSFC)
Power frequency 1
Temper Quench Quench Off Cycle time
Final heat frequency 2
Final heat Preheat
Load On Off
On Cycle time
Fig.13. Concepts of gear hardening by induction.Heat Treatment of Metals 2004.1
Induction Hardening of Gears: a Review
Fig.14. (a) Equipment used to harden OD and ID of gears such as that in (b). (Courtesy of Inductoheat Inc.).
place, using an integrated quench. A third technique requires the use of a separate concentric quench block (quench ring) located below the inductor. It has been reported11,14 that more favourable compressive stresses within the tooth root were achieved with the gear spin hardening technique than with the tooth-by-tooth or gap-by-gap methods. Fig.13 shows three of the most popular design approaches for induction gear heat treating processes that employ encircling-type coils: conventional single-frequency concept (CSFC); pulsing single-frequency concept (PSFC); and pulsing dual-frequency concept (PDFC). All three can be used in either a single-shot or scanning mode. Conventional Single-Frequency Concept (CSFC) The conventional single-frequency concept1,7 is used for hardening gears with medium and small teeth. As seen in Fig.3 (patterns B and E), the teeth are often throughhardened. Quite frequently, CSFC can also be used successfully for medium-size gears. As an example, Fig.14a shows an induction gear hardening machine that applies this approach. The gear being heat treated in this application is an automotive transmission component with helical teeth on the inside diameter (ID) and large teeth on the outside diameter (OD) for a parking brake. Both the inside and outside diameters require
hardening (Fig.14b). The hardening of the ID gear teeth requires a higher frequency than the OD. Therefore a frequency of 10kHz was chosen for OD heating and 200kHz was selected for ID heating. Subsequently, quenchant is applied to the hot gear in place; that is, no repositioning is required. This practically instantaneous quench provides a consistent metallurgical response. During quenching, there is minimal or no rotation to ensure that the quenchant penetrates all areas of the gear evenly. With the equipment in Fig.14a, gears conveyed to the machine are transferred by a cam-operated robot to the heat-treating station. Parts are monitored at each station and accepted or rejected based on all the major factors that affect hardened gear quality. These include energy input into the part, quench flow rate, temperature, quench pressure and heat time. An advanced control/monitoring system verifies all machine settings to provide confidence in the quality of processing for each individual gear. Precise control of the hardening operations, and careful attention to the coil design, minimise part distortion and provide the desirable residual stresses in the finished gear. The hardened gear is inspected and moved to the next operation. Although CSFC is most suitable for small- and medium-size gears, there are cases when this concept can also be used successfully for large gears. For example, Fig. 15 shows an induction machine where a multi-turn encircling inductor is used for hardening gears with a major diameter of 701mm, root diameter 617mm and thickness 79mm. In this particular case, it was in the users best interest to harden and temper in the same coil using the same power supply. In other cases, this might not be the best solution. In order to prevent problems, such as pitting, spalling, tooth fatigue and poor endurance, hardening of the contour of the gear (contour hardening) is quite often required. In some cases, this can be a difficult task due to the difference in current density (heat source) distribution and heat-transfer conditions within a gear tooth. Two main factors complicate the task of obtaining the required contour-hardened profile. With encircling-type coils, the root area does not have good coupling with the inductor compared with that at the gear tip. Therefore, it is more difficult to induce energy into the gear root. In addition, there is a significant heat sink located under the gear root (below the base circle, Fig.4). Pulsing Single-Frequency Concept (PSFC) In order to overcome these difficulties, and to be able to meet customer specifications, the pulsing single-frequency concept was developed (Fig.13b). In many cases, PSFC allows the user to avoid the shortcomings of CSFC andHeat Treatment of Metals 2004.1
Fig.15. Induction equipment for hardening large gears. (Courtesy of Inductoheat Inc.). 12
V. Rudnev, D. Loveless, R. Cook and M. Black
obtain a contour hardening profile. Pulsing provides the desirable heat flow toward the root of the gear without noticeable overheating of the tooth tip. A well-defined crisp hardened profile that follows the gear contour (patterns F and G in Fig.3) can be obtained using high power density at the final heating stage. A typical dual-pulse contour hardening system, which applies a pulsing single-frequency concept, has been discussed1,15,16. This machine is designed to provide gear contour heat treatment (including preheating, final heating, quenching and tempering) with the same coil, using one high-frequency power supply. Fig.13b illustrates the process cycle with moderate-power preheat, soaking stage, short high-power final heat and quench, followed by lowpower heat for temper. Preheating ensures a reasonable heated depth at the roots of the gear, enabling the attainment of the desired metallurgical result and decreasing the distortion in some materials. Preheat times are typically from several seconds to a minute, depending on the size and shape of the gear. Obviously, preheating reduces the amount of energy required in the final heat. After preheating, there might be a soak time, ranging from 2 to 10 seconds, to achieve a more uniform temperature distribution across the teeth of the gear. Final heat times can range from less than one second to several seconds. As a general rule, for both CSFC and PSFC techniques, the higher frequency is called for by finer-pitch gears, which typically require a shallower case depth. Fig.16a shows a unitised induction hardening system, capable of providing both CSFC and PSFC gear hardening, and Fig.16b illustrates a double sprocket hardened therein. Pulsing Dual-Frequency Concept (PDFC) A third approach, the pulsing dual-frequency concept, is not new. The idea of using two different frequencies to produce the desired con